1 / 41

# Analysis of Materials Polymers by Thermal Methods: DSC, TG - PowerPoint PPT Presentation

Analysis of Materials (Polymers) by Thermal Methods: DSC, TG/DTA Instructor: Ioan I. Negulescu CHEM 4010 Tuesday, October 29, 2002. Thermal Methods:

I am the owner, or an agent authorized to act on behalf of the owner, of the copyrighted work described.

## PowerPoint Slideshow about 'Analysis of Materials Polymers by Thermal Methods: DSC, TG' - dayo

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -
Presentation Transcript

DSC, TG/DTA

Instructor: Ioan I. Negulescu

CHEM 4010

Tuesday,

October 29, 2002

Thermal methods are based upon the measurement of the dynamic relationship between temperature and some property of the system such as mass and heat absorbed or evolved by/from it.

DSC

Differential Thermal Analysis,

DTA

Thermogravimetry,

TG

are the most important thermal methods

used in characterization of polymers.

The temperature increase, T, of a body which is heated is directly proportional to the amount of heat absorbed, Q, and inversely proportional to its mass, m, and its capacity C to store heat:

T = Q/m C Eq. 1

Consider the temperature increase of two different samples of the same mass

m1 = m2

for which the same amount of heat was given

Q1 = Q2

If their heat capacities are different

C1 C2

they do not experience the same temperature increase, i.e.,

T1T2

A greater heat flow (dQ/dt, where t is time) of the same mass

will always flow into the sample whose heat capacity is higher, in order that the steady-state heating rate be maintained.

The heat capacity at constant pressure (Cp)

of a material is defined as the temperature increase of a unit of substance (mass) as a result of the supply of a unit of heat at

constant pressure.

For the same substance, C of the same massp is dependent upon its aggregation state, i.e., it is different for the liquid state as compared to loose gaseous or to more compact solid state.

A polymeric material has different heat capacities for amorphous or crystalline morphologies. For amorphous polymers, the heat capacity for the glassy state (i.e., below glass transition, Tg, where only vibrations of atomic groups occur) is different from that characterizing the leathery (short range diffusional motion, i.e., of chain segments), rubbery (retarded long-range motions), rubbery flow (slippage of long-range entanglements) or liquid state.

Figure 1. Temperature - molecular mass diagram for amorphous polymers: (1) Glass transition (Tg); (2) Diffuse transition zone; and (3) Thermal decomposition.

Figure 2. Temperature - Molecular Mass diagram for (semi) -crystalline polymers: (1) Glass transition (Tg); (2) Melting point (Tm); (3) Diffuse transition zone; and (4) Thermal decomposition.

For amorphous polymers, the glass-rubber transition temperature is of considerable importance technologically. It (Tg) determines the lower use limit of a rubber (e.g., polydienes, Tg -50°C) and the upper limit use of an amorphous thermoplastic material(e.g., polystyrene, Tg 100 ° C).

In the case of (semicrystalline) linear polymers it is possible to identify a melting temperature (Tm). Above this temperature the polymer may be liquid, viscoelastic or rubbery according to its molecular mass, but below it, at least in the high molecular mass range, it will tend to be leathery and tough down to the glass transition temperature.

POLYHYDROXYALKANOATES possible to identify a

R can be hydrogen or hydrocarbon chains of up to

around C13 in length, and x can range from 1 to 3 or

more. Varying x and R effect hydrophobicity, Tg, Tm,

and level of crystallinity

Fig 4: The Family of PHAs has Physical Characteristics that possible to identify a

Allow it to be Used Across a Wide Spectra of Applications

POLYHYDROXYALKANOATES

Detailed information on glass transition, crystallization, and melting, is therefore critically important in formation, processing and utilization of polymers.

Differential thermal methods (DTA and DSC) have been widely applied to the study and characterization of polymeric materials.

In DTA the heat absorbed or emitted by a system is observed by measuring the temperature difference (T) between that system (the sample) and an inert reference material (often alumina), as the temperature of both is increased at a constant rate (usually 5-10 C/min).

Figure 3. Schematic diagram of a typical DTA apparatus. by measuring the temperature difference (

In DSC, the sample and the reference are also subjected to a continuously increasing or decreasing temperature.

In the scanning operation the sample and the reference show different temperature independent heat capacities.

Heat (dQ/dt) is added to the sample or to the reference as necessary to maintain the two identical temperatures.

Bottom: (b) measured curve. a continuously increasing or decreasing temperature.m is the measured heat flux. bl is the heat flux corresponding to the base line and t is time.

The ordinate is usually represented by the heat flux (denominated as  or dQ/dt) or by the variation of the heat capacity.

The glass-to-rubber transition, or shortly the glass transition (Tg) is a phase change reminiscent of a thermodynamic second order transition (melting and crystallization being first order transitions) for which a plot of specific heat versus temperature shows a sudden jump.

The first order transitions appear

as peaks.

DSC curve of a polymeric sample: (1), (3) and (5) are base lines; (2) is glass-to-rubber transition, Tg; (4) is the interpolated base line; and (6) is the first order transition peak.

The glass transition region in cooling (a) and subsequent heating (b) mode showing some commonly used definitions of glass transition, Tg.

Poly(Lactic Acid) heating (b) mode showing some commonly used definitions of glass transition, T

• -[-O-CH(CH3)-CO-]n

• Two of the most attractive features of

• poly(lactic acid), PLA, polymers are:

• they are easily synthesized from

• renewable resources (corn!)

• they are both hydro- and biodegradable

Poly (Lactic Acid) heating (b) mode showing some commonly used definitions of glass transition, T

Glass transition temperature, Tg.

DSC traces for melting and crystallization heating (b) mode showing some commonly used definitions of glass transition, T

of a polymer sample.

Melting of polyoxymethylene with superheating. heating (b) mode showing some commonly used definitions of glass transition, T

DSC traces of Low Crystallinity PLA treated in Water at 70 quenched from the melt.C and 100C. The higher the crystallinity achievedat 100 C, the higher and the less defined the Tg

Considering quenched from the melt.H = 200 mJ/mg as the enthalpic change for the melting of a 100% crystalline HDPE sample, from DSC data of these two recyclable HDPE it can be found that:

the polymer derived from detergent bottles was (132/200)x100 = 66% crystalline

the polymer used for milk bottles was (165/200)x100 = 82.5% crystalline.

Polyhydroxylated Nylons filler from DSC data.

Similarity of Nylon 6,6 and the poly hydroxylated counterpart:

DSC Thermal Transitions in Polyhydroxylated filler from DSC data.

Nylon 6,6

Thermogravimetric (TG) analysis filler from DSC data. is concerned with the change in weight of a material as its temperature changes. This indicates:

the temperature at which the material loses weight through evaporation or decomposition

the temperature at which no weight loss takes place is revealed, which indicates stability of the material.

Thermal Degradation of Polyhydroxylated filler from DSC data.

Nylon 6,6

Poly (4-dodecyl-1-4-aza heptamethylene-D-glucaramide). filler from DSC data.

Thermal decomposition.

Initial decomposition of linear polymers. filler from DSC data.

Initial sample weight: 10 mg. Heating rate: 5C/min.

Thermogravimetric analysis of a polymeric blend containing HDPE and an inorganic filler (phosphogypsum)

Almost any measurement that can be done at different temperatures can be expanded into thermal analysis; and any series of thermal analysis techniques can be combined with other non-thermal technique for valuable multiple-parameter information.

Coupled techniques, such as Thermogravimetry, Differential Thermal Analysis and Mass Spectrometry (TG-DTA-MS) or evolved gas analysis of polymers by coupled Thermogravimetry, Gas Chromatography, Fourier Transform Infrared and Mass Spectrometry (TG-GC-FTIR-MS) are just two examples often used in industrial laboratories.